Table 11. Continued 



Alloy 



CDA No." 



Environment 



Exposure 

 (day) 



Depth 

 (ft) 



Corrosion 

 Rate 



(mpy) 



Type of 

 Corrosion^ 



Source 



Copper, free 



102 



W 



197 



2,340 



1.4 



U 



INCO (3) 



Copper, O free 



102 



S 



197 



2,340 



0.2 



U 



CEL (4) 



Copper, free 



102 



S 



197 



2,340 



0.2 



u 



INCO (3) 



Copper, O free 



102 



W 



402 



2,370 



0.9 



u 



CEL (4) 



Copper, O free 



102 



w 



402 



2,370 



1.4 



u 



INCO (3) 



Copper, O free 



102 



s 



402 



2,370 



0.6 



u 



CEL (3) 



Copper, O free 



102 



s 



402 



2,370 



0.2 



ET 



INCO (3) 



Copper, O free 



102 



w 



181 



5 



1.4 



P(22m) 



CEL (4) 



Copper, free 



102 



w 



181 



5 



1.8 



G 



INCO (3) 



Copper, free 



102 



w 



366 



5 



1.2 



G 



INCO (3) 



Copper, O free^ 



102 



w 



386 



5 



0.7 



U 



MEL (5) 



Copper, O free 



102 



w 



398 



5 



1.1 



G, P(37m) 



CEL (4) 



Copper, free 



102 



w 



540 



5 



0.9 



G, P(22m) 



CEL (4) 



Copper, free 



102 



w 



588 



5 



0.9 



G, P (20m) 



CEL (4) 



Be-Cu^ 



170 



w 



123 



5,640 



0.5 



U 



NADC (7) 



Be-Cu 



170 



w 



751 



5,640 



0.5 



U 



NADC (7) 



Be-Cu 



170 



w 



197 



2,340 



0.0 



NC 



NADC (7) 



Be-Cu 



170 



w 



402 



2,370 



0.6 



u 



NADC (7) 



Be-Cu 



172« 



w 



123 



5,640 



0.5 



u 



NADC (7) 



Be-Cu 



172 h 



w 



123 



5,640 



0.5 



u 



NADC (7) 



Be-Cu 



172* 



w 



751 



5,640 



0.5 



u 



NADC (7) 



Be-Cu 



172 fc 



w 



751 



5,640 



0.5 



u 



NADC (7) 



Be-Cu 



172* 



w 



197 



2,340 



0.2 



u 



NADC (7) 



Be-Cu 



ll2 h 



w 



197 



2,340 



0.2 



u 



NADC (7) 



Be-Cu 



172* 



w 



402 



2,370 



0.5 



u 



NADC (7) 



Be-Cu 



172* 



w 



402 



2,370 



0.4 



u 



NADC (7) 



Be-Cu 



172 



w 



402 



2,370 



0.6 



u 



CEL (4) 



Be-Cu 



172 



s 



402 



2,370 



0.5 



u 



CEL (4) 



Be-Cu 



172 



w 



181 



5 



0.1 



u 



CEL (4) 



Be-Cu 



172 



w 



364 



5 



1.1 



u 



CEL (4) 



Be-Cu 



172 



w 



723 



5 



0.8 



u 



CEL (4) 



Be-Cu 



172 



w 



763 



5 



0.8 



u 



CEL (4) 



Be-Cu 





172 



w 



402 



2,370 



0.5 



\jj 



CEL (4) 



Be-Cu 





172 



s 



402 



2,370 



0.5 



u' 



CEL (4) 



Be-Cu 





172 



w 



181 



5 



0.1 



u' 



CEL (4) 



Be-Cu 





172 



w 



364 



5 



1.0 



u 



CEL (4) 



Be-Cu 





172 



w 



723 



5 



0.7 



u 



CEL (4) 



Be-Cu' 



172 



w 



763 



5 



0.8 



u 



CEL (4) 



Be-Cu* 



172 



w 



402 



2,370 



0.6 



ET 



CEL (4) 



Be-Cu* 



172 



s 



402 



2,370 



0.5 



ET 



CEL (4) 



Continued 



58 



